Rubber recovery from centrifuged natural rubber latex ...
Embed Size (px)
Transcript of Rubber recovery from centrifuged natural rubber latex ...
Rubber recovery from centrifuged natural rubber latex residueusing sulfuric acid
Department of Materials Science and Technology, Faculty of Science,Prince of Songkla University, Hat Yai, Songkhla, 90110 Thailand.
Received 12 April 2012; Accepted 16 January 2013
Waste latex sludge from centrifuged residue, which is a null by-product of concentrated latex manufacturing, wasdigested to retrieve the rubber by using sulfuric acid. It was found that the acid concentration and digestion time have aneffect on the amount and purity of the retrieved rubber. Sulfuric acid at concentrations of more than 10% by weight with adigestion time of 48 hours completely digested waste latex sludge and gave rubber 10% by weight. The quality of the retrievedrubber was examined for Mooney viscosity (MV), plasticity retention index, nitrogen content, and ash content. The averagemolecular weight of the retrieved rubber, using gel permeation chromatography, was lower than that of normal natural rubber(NR) which corresponds with the MV and initial plasticity (Po). The molecular structure from Fourier transform infraredspectroscopy (FT-IR) indicated that the retrieved rubber surface is wet composed with hydroxyl functional ended group.The residue solution was evaporated and crystallized. The structure of crystals was determined using power X-ray diffracto-meter.
Keywords: waste latex sludge, concentrated latex, rubber recovery, Boussingaultite
Songklanakarin J. Sci. Technol.35 (2), 213-216, Mar. - Apr. 2013
Concentrated natural rubber latex (NRL) is usuallyproduced by using centrifugation of fresh field NRL. NRL isnot only consisted of natural rubber (NR) particles but alsonon-rubber parts such as magnesium (Mg). The NRL canshow high Mg contents, which have an impact to the centri-fugation process and the quality of concentrated latex.Therefore, it is necessary to remove the magnesium fromNRL. The traditional method is adding diammonium hydro-gen phosphate (DAHP) to NRL and leaving it for more than12 hours. The reaction of DAHP with Mg results in solidsludge formation and precipitation. The solid sludge charac-teristics have been investigated and their advantages foragronomic relevance have been reported since 2002(Okieimen et al., 2002). Basic composition of this materials
are rubber hydrocarbon, nitrogen, magnesium, and phospho-rus with 12.5%, 3.3%, 12.2%, and 14.7% by wt. (dry weight),respectively (Boonsawang et al., 2008). Even though thesematerials can be also used as commercial phosphatic fertili-zers (Tekprasit, 2000), it has limitations, due to heavy metalcontent, as well as the unsuitability to certain soils and cropsmust be concerned. Additionally, rubber hydrocarbon is noteasily decomposed in soils. Commonly, the waste sludgefrom waste water treatment plants was digested using acid(Pearson and Buswell, 1931) for different purposes such asammonia removal (Suschka and Poplawski, 2004) andphosphorus recovery (Stark, 2002). In this paper, the aciddigestion of waste latex sludge from centrifugation was inves-tigated for the recovery of the rubber and the occurrence ofhigh purity ammonium magnesium sulfate.
The sludge, collected form a latex centrifuge machine,was kindly supplied by Chalong Concentrated Latex Com-
* Corresponding author.Email address: [email protected]
W. Taweepreda / Songklanakarin J. Sci. Technol. 35 (2), 213-216, 2013214
pany Limited and was used immediately after. The sludge wasgrinded into small pieces as shown in Figure 1. Grind sludgewas weighted for 300 grams before mixing with differentsulfuric acid concentrations (5%, 10%, 20%, 30%, and 40%by wt.) for 600 mL. The sulfuric acid was selected as it is verycheap and strong enough to remove non-rubber componentswith low recovery cost. Acid digestion reduced the volumeof sludge and decomposed of inorganic substance results infloating retrieved rubber at room temperature. The volume ofsludge was decreased with increasing the acid concentrationdue to decomposition of organic sludge which was convertedinto gases. The sulfuric acid for 5% by wt. was not strongenough to remove non-rubber component from the wastesludge. The sludge was still precipitated due to high densityas illustrated in Figure 2. The sludge digestion with high acidconcentration resulted in low pH waste water and acid con-taminated in retrieved rubber. The retrieved rubber with highacid contamination has poor properties. In this experiment,the rubber recovery with 10% by wt. sulfuric acid digestionwas selected.
The retrieved rubber was separated, washed withwater, sheeted, and dried in an air oven at 70ºC. The composi-tion of the retrieved rubber was analyzed using Thermogravi-metric Analyzer (TGA) (PerkinElmer, TGA7) comparing withthat of waste sludge. The rubber structure and molecularweight were characterized using Fourier Transform InfraredSpectrometer (FT-IR) Model EQUINOX 55 (Bruker) and Gelpermeation chromatography (GPC) (SHIMUDZU), respec-tively. Quality of the retrieved rubber was characterized andcompared with standard NR which is classified in STR5Lgrade such as Mooney viscosity (MV), plasticity retentionindex (PRI), nitrogen and ash content. The Mooney viscositywas determined by Mooney viscometer (ALPHA Tech.,MV2000) with large rotor at 100ºC. The Mooney viscositywas measured according to ISO 289. This standard specifiesthe test temperature, sample preheating time before the startof shearing (1 min) and shearing duration (4 min). TheMooney viscosity was reported in Mooney Unit (MU). Atleast three samples were used for the experiment. The initialplasticity and plasticity retention index were measuredaccording to ISO 2930. Six test-pieces were died out fromdoubled sheets with the Wallace punch. The average thick-ness of the test-pieces was 3.4±0.2 mm. They were randomlydivided into two sets of three, one set for plasticity testsbefore aging and the other for testing after aging for 30 minat 140ºC. After that, the test-pieces were removed from theoven. Then they were allowed to cool down to room tem-perature for a minimum of 30 min and after that plasticity (P30)was measured. The PRI was estimated by the percentage ratiobetween P30 and P0 as given in Equation 1. The nitrogen andash content were measured according to ISO 1656 and ISO247, respectively.
The residue waste water was characterized and wascrystallized at room temperature. The crystal structure wascharacterized by using X-ray Diffractometer (X’Pert MPD,Philips, Netherlands).
3. Results and Discussion
The compositions of waste latex sludge and retrievedrubber from TGA is illustrated in Figure 3. The waste latexsludge composed of moisture, rubber hydrocarbon and in-organic substance with 35%, 20%, and 45% by wt., respec-tively. Acid digestion released most of the bound water inthe sludge and the retrieved rubber composed of more than95% by wt. of rubber. Most of the inorganic substances weredecomposed and dissolved in the solution of sulfuric acid.
Figure 1. Waste latex sludge before (a) and after grinding (b).
Figure 2. Effect of the sulfuric acid concentration on the sludge di-gestion.
Figure 3. TGA thermogram of solid sludge before and after diges-tion with sulfuric acid.
215W. Taweepreda / Songklanakarin J. Sci. Technol. 35 (2), 213-216, 2013
The FT-IR spectra of the retrieved rubber comparedwith standard NR (STR5L) is shown in Figure 4. The majorcharacteristic peaks of standard NR are at 2962 cm-1 (CH3asymmetric stretching), 2855 cm-1 (CH2 asymmetric stretch-ing), 1650 cm-1 (C=C stretching), 889 cm-1 (CH3 wagging), and837 cm-1 (=C-H wagging). For the retrieved rubber, the occur-rence of a peak at 713 cm-1 (O-H out-of-plane bend) and abroader peak at 3340 cm-1 (hydroxyl group, H-bonded OHstretch) indicating a higher number of water moleculessurrounding the membrane and the functional ended groupof the retrieved rubber might be hydroxyl and carbonyl(Santos et al., 2005).
The GPC result of the retrieved rubber as shown inFigure 5 found that the average molecular weight by number(Mn) and the average molecular weight by weight (Mw) of theretrieved rubber are 90,000 and 313,000 g/mol, respectively.The molecular weight, representing the rubber moleculechain length, of the recovered rubber from sludge is very lowcompared with the standard NR (Mn = 442,400 g/mol, Mw =1,745,500 g/mol).
Figure 6. Crystals from residue solution.
Figure 7. Powder X-ray diffraction patterns of the retrieved crystals.
Table 1. Properties of retrieved rubber from solid sludge
STR 5L Retrieved rubber
Mooney Viscosity [ML1+4, 100°C] 60 49Initial Plasticity (Po) 40 33Plasticity Retention Index (PRI) 77 93Nitrogen content (%) 0.3 0.9Ash content (%) 0.1 3.5
contamination with natural anti-oxidants. The results of thisstudy hold promise as an apparent feasible solution to theproblem of waste disposal in the NR latex concentratingfactories with cost effectiveness and also gains valued NRfrom waste sludge, which is usually a cheap throw awaymaterial.
The waste water from sludge digestion with 10% bywt. sulfuric acid is dark brown in color with a pH = 5.8; it wasanalyzed for BOD and COD. The results found that the BODand COD were 2,200 and 27,200 mg/L, respectively. Theresidue digestive was concentrated by evaporation at 100ºCand allowed crystal formation at room temperature.
The occurred crystals are white to clear in color andthe gloss is vitreous as shown in Figure 6. The powder X-raydiffraction pattern of the crystals as shown in Figure 7 werein good agreement with Boussingaultite mineral (RRUFFID- R070597.9) (Margulis et al., 1962) and the refine unit cellparameters are a=9.327(3) Å, b=12.600(4) Å, c=6.210(1) Å,b=107.091(6)o, and V=697.6(8) Å3 (Shimobayashi et al., 2011).
Figure 4. FT-IR spectra of retrieved rubber and standard NR(STR5L).
Figure 5. GPC chromatogram of the retrieve rubber.
The rubber properties of the retrieved rubbercompared with standard NR (STR5L) is illustrated in Table 1.The Mooney viscosity and initial plasticity of the retrievedrubber are lower than that of standard NR due to the lowmolecular weight of retrieved rubber. But the PRI of retrievedrubber is higher than that of standard NR indicated that theretrieved rubber is not easily oxidation degraded because of
W. Taweepreda / Songklanakarin J. Sci. Technol. 35 (2), 213-216, 2013216
The rubber removal from waste sludge using sulfuricacid is a feasible solution to solve the problem of wastedisposal in the NR latex concentrating factories in any de-veloping country like Thailand. The process is not onlyretrieving high value NR but also magnesium ammoniumsulfate, which is an essential nutrient in crop production;both retrieved form a throw away material.
The authors are grateful to the financial supportsfrom the Office of National Research Council of Thailand(NRCT) (Project code: 50860).
Boonsawang, P., Laeh, S. and Intrasungkha, N. 2008. En-hancement of sludge granulation in anaerobic treat-ment of concentrated latex wastewater. Songklanaka-rin Journal of Science and Technology, 30 (Suppl. 1),111-119.
Dos Santos, K.-A.-M., Suarez, P.-A.-Z. and Rubim, J. C. 2005.Photo-degradation of synthetic and natural polyiso-prenes at specific UV radiations. Polymer Degradationand Stability. 90, 34-43.
Liu, X., Du, G. and Chen, J. 2008. Enhancement of solubilisa-tion and acidification of waste activated sludge bypretreatment. Waste Management. 28, 2614-2622.
Margulis, T.-N. and Templeton, D.-H. 1962. Crystal structureand hydrogen bonding of magnesium ammoniumsulfate hexahydrate, Zeitschrift für Kristallographie.117, 344-357.
Okieimen, C.-O. and Okieimen, F.-E. 2002. Effect of naturalrubber processing sludge on the degradation of crudeoil hydrocarbons in soil. Bioresource Technology. 82,95-97.
Pearson, E.-L. and Buswell, A.-M. 1931. Acid Sludge Diges-tion. Industrial & Engineering Chemistry. 23(10), 1144-1145.
Sakohara, S., Yagi, S. and Iizawa, T. 2011. Dewatering of in-organic sludge using dual ionic thermosensitive poly-mers. Separation and Purification Technology. 80, 148-154.
Shimobayashi, N., Ohnishi, M. and Miura, H. 2011. Ammo-nium sulphate minerals from Mikasa, Hokkaido, Japan:boussingaultite, godovikovite, efremovite and tscher-migite. Journal of Mineralogical and PetrologicalScience 106, 158-163.
Stark K. 2002. Phosphorus release from sewage sludge by useof acids and bases. Licentiate Thesis, Department ofLand and Water Resources Engineering, KTH,Stockholm, Sweden, ISBN 91-7283-307-6.
Suschka, J., Poplawski, S. 2004. Ammonia removal from di-gested sludge supernatant In Plaza, Levlin, Hultman,editors, Integration and optimisation of urban sanita-tion systems. TRITA-LWR.REPORT 3007, Report No11, pp. 113-120.
Tekprasit, V. 2000. The Utilization of the Centrifuged Residuefrom Concentrated Latex Industry as a Soil Condi-tioner. M.Sc. Thesis. Prince of Songkla University (inThai).